Contents lists available atScienceDirect
Characterisation of a high pH cement back
ll for the geological disposal of
nuclear waste: The Nirex Reference Vault Back
Rita G.W. Vasconcelosa
, Nicolas Beaudoinb,c
, Andrea Hamiltonb
, Neil C. Hyatta
, John L. Provisa
Claire L. Corkhilla,∗
aNucleUS Immobilisation Science Laboratory, Department of Materials Science and Engineering, University of Sheﬃeld, S1 3JD, UK bDepartment of Civil and Environmental Engineering, University of Strathclyde, Glasgow, G1 1XJ, UK
cSchool of Geographical and Earth Sciences, University of Glasgow, Glasgow G12 8QQ, UK
A R T I C L E I N F O
Handling Editor: Prof. M. Kersten
Geological disposal Nuclear waste Cement Mineralogy Microstructure
A B S T R A C T
In a conceptual UK geological disposal facility for nuclear waste within a high-strength, crystalline geology, a cement-based backﬁll material, known as Nirex Reference Vault Backﬁll (NRVB), will be used to provide a chemical barrier to radionuclide release. The NRVB is required to have speciﬁc properties to fulﬁl the opera-tional requirements of the geological disposal facility (GDF); these are dependent on the chemical and physical properties of the cement constituent materials and also on the water content. With the passage of time, the raw materials eventually used to synthesise the backﬁll may not be the same as those used to formulate it. As such, there is a requirement to understand how NRVB performance may be aﬀected by a change in raw material supply. In this paper, we present a review of the current knowledge of NRVB and results from a detailed characterisation of this material, comparing the diﬀerences in performance of theﬁnal product when diﬀerent raw materials are used. Results showed that minor diﬀerences in the particle size, surface area and chemical composition of the raw material had an eﬀect on the workability, compressive strength, the rate of hydration and the porosity, which may inﬂuence some of the design functions of NRVB. This study outlines the requirement to fully characterise cement backﬁll raw materials prior to use in a geological disposal facility and supports ongoing assessment of long-term post-closure safety.
Intermediate Level Waste (ILW) comprises a signiﬁcant proportion, approximately 450 000 m3, of the UK's projected inventory of
radio-active waste (Nuclear Decommissioning Authority, 2015). This includes waste arising from the reprocessing of spent nuclear fuel (e.g. spent fuel cladding) and from the operation, maintenance and decommissioning of nuclear facilities (e.g. sludges from the treatment of radioactive li-quid eﬄuents) (Hicks et al., 2008). This waste is destined for ﬁnal disposal in a Geological Disposal Facility (GDF) (Nuclear Decommissioning Authority, 2010a), where the conditioned waste packages will be placed in vaults excavated in host rock, deep under-ground (Nuclear Decommissioning Authority, 2010b). In a conceptual scenario where a high-strength crystalline rock will host the facility, the vaults will be backﬁlled with a cement-based material to provide a physical and chemical barrier to radionuclide release (Nuclear Decommissioning Authority, 2010b). For this purpose, the Nirex Re-ference Vault Backﬁll (NRVB) has been considered (Francis et al.,
NRVB was designed in the 1990s to fulﬁl a number of speciﬁc re-quirements for use in a UK geological disposal facility (Francis et al., 1997; Hooper, 1998). These include (Crossland and Vines, 2001; Nuclear Decommissioning Authority, 2010c; United Kingdom Nirex Limited, 2005):
- providing a high alkaline buﬀered environment, through the dis-solution of the diﬀerent cement hydrate phases by groundwater, to suppress dissolved concentrations of many radionuclides;
- possessing high permeability and porosity to ensure homogeneous chemical conditions, to allow the escape of the gases generated in the GDF and to provide a high surface area for radionuclide sorp-tion; and
- exhibiting low strength to facilitate the possibility of re-excavation of the vaults, if required.
Despite an initial assessment of NRVB at the time of the design and
Received 21 July 2017; Received in revised form 3 October 2017; Accepted 14 November 2017 ∗Corresponding author.
E-mail address:c.corkhill@sheﬃeld.ac.uk(C.L. Corkhill).
Available online 15 November 2017
patent (Francis et al., 1997), and subsequently, several assessments of various aspects of this material (e.g. mineralogy, strength, or porosity, as described below), there has not been a comprehensive character-isation of NRVB, where all tests are performed on a consistent batch. Additionally, some of the raw materials used in early development of NRVB are no longer available due to changes in the powder suppliers (Radioactive Waste Management, 2016), therefore, materials to be used when a GDF is in operation may diﬀer in composition and other key characteristics. It is important to understand how the chemical and physical properties of the backﬁll raw materials may aﬀect the short-and long-term performance of the backﬁll, to support development of GDF engineering and post-closure safety assessment. We here present a literature review of the published data on NRVB, even where datasets are incomplete, or details pertinent to the analysis of the data are ab-sent.
1.1. NRVB hydration
Portland cement (PC), calcium hydroxide [Ca(OH)2] and calcium
carbonate (CaCO3) are the main components of NRVB (Hooper, 1998).
The original formulation used a water/solid ratio (w/s) of 0.55 and a water to cement (w/c) ratio of 1.367. According to this composition, Holland and Tearle (2003)described the expected mineralogy of NRVB and the respective changes in relation with temperature. Theoretically, at ambient temperature, the phase assemblage of NRVB is expected to contain calcium hydroxide (also known as portlandite), calcite (CaCO3),
calcium silicate hydrate (C-S-H), AFt (ettringite) and AFm (mono-carboaluminate) phases, and possibly hydrotalcite if magnesium car-bonate is present in the limestone ﬂour or in the Portland cement (Holland and Tearle, 2003). At high temperatures (80 °C), the forma-tion of hydrogarnet-type phases was also predicted, according to ther-modynamic modelling (database not speciﬁed) performed by the same authors (Holland and Tearle, 2003), although more recent advances in cement chemistry and phase assemblage prediction models indicate that this may be less likely due to the high quantity of carbonate present in this cement formulation. Experimental X-ray diﬀraction (XRD) per-formed on fresh (uncured) NRVB revealed that the main phase present was calcite, whereas for NRVB cured for 4 months and 3 years, the phase assemblage was dominated by portlandite (Felipe-Sotelo et al., 2012).
Portlandite and C-S-H are expected to provide the high alkaline-buﬀering capacity of NRVB. It is proposed that when the backﬁll ma-terial isﬁrst in contact with groundwater, the pH will be buﬀered by the dissolution of the more soluble phases, alkali (i.e. Na, K) hydroxides and sulfates. After the removal of the alkali metal salts, buﬀering will continue through the dissolution of portlandite; a solution saturated with respect to portlandite is formed with a pH of about 12.5 at 25 °C (Francis et al., 1997). After the portlandite has been exhausted, pH buﬀering will be maintained by the incongruent dissolution of C-S-H phases with relatively high calcium/silicon molar ratios (Ca/Si), around 1.5. From this, dissolution will result in the release of calcium and hydroxide ions, thus lowering the Ca/Si ratio and reducing the pH value at which the water is buﬀered (Harris et al., 2002; Hoch et al., 2012). The buﬀering timescale and capacity of NRVB will depend mainly on the composition and rate of groundwater leaching (Bamforth et al., 2012; Francis et al., 1997). According to a recent study regarding the leaching behaviour of C-S-H using demineralised water, even with a low Ca/Si ratio, the dissolution of C-S-H will buﬀer the pH to∼10 (Swanton et al., 2016).
1.2. Physical properties of NRVB
The physical properties of NRVB were summarized byFrancis et al. (1997) andBamforth et al. (2012). The compressive strength of the NRVB (w/s = 0.55) was found to be 4.9 MPa, 5.9 MPa and 6.3 MPa after 7, 28 and 90 days of curing respectively (Francis et al., 1997).
When comparing with compressive strength values obtained for Port-land cement (w/s = 0.50), (e.g. 31 MPa, 45 MPa and 46 MPa after 7, 28 and 90 days, respectively, fromMenéndez et al. (2003)), the values obtained for NRVB are very low. This relatively low strength thus al-lows retrievability of waste packages from within NRVB-backﬁlled vaults (Crossland and Vines, 2001; Nuclear Decommissioning Authority, 2010c; United Kingdom Nirex Limited, 2005).
Since the repository operating temperatures will be higher than the 20 °C used for standard cement curing, studies have been performed to assess the eﬀect of curing temperature (30 °C, 60 °C and 90 °C, cured in moist or excess volume of water) on the strength of NRVB (Francis et al., 1997). Results showed that increasing the temperature of curing corresponds to a reduction in the strength, for example after 28 days of curing at 90 °C, the compressive strength was halved when compared to curing at 30 °C (Francis et al., 1997). Similar results have been obtained with Portland-limestone cement, where a temperature increase nega-tively inﬂuenced compressive strength (Lothenbach et al., 2007). It should be noted, however, that such high curing temperatures (90 °C) are not expected within a GDF vault for ILW.
1.3. Microstructural properties of NRVB
Porosity and permeability must be carefully considered when de-signing a cementitious material for a GDF, since these properties will inﬂuence the transport characteristics of groundwater and radionuclide species through the cement. For example, having a high porosity (more than 30%) allows the ingress of groundwater, dissolution of the dif-ferent hydrate phases, so providing a high alkaline environment. It also allows the diﬀusion of gases produced in the waste packages and gives rise to a high surface area, capable of sorbing radionuclide species.
NRVB is relatively porous; the total porosity of NRVB includes a high quantity of unreacted material, was reported to be 50% using mercury intrusion porosity and nitrogen desorption methods, at an unspeciﬁed curing age (Francis et al., 1997). However by, comparing the density obtained in dry and water conditions by Francis et al., we can calculate the porosity to be 35%. X-ray computed tomography (XCT) gave a segmented porosity of∼40% for large scale samples in the non-carbonated region of an NRVB-carbonation trial (Heyes et al., 2015).
After closure, the formation of gases is expected to occur in the GDF, e.g. from corrosion of Magnox cladding, fuel fragments, uranium and steel under anaerobic conditions, microbial degradation of organic compounds and radiolysis of water (Harris et al., 1992). As a result, the permeability of NRVB should be suﬃcient to allow gas movement without signiﬁcant over-pressurisation and cracking (Francis et al., 1997). The gas permeability coeﬃcient for argon and helium in NRVB at 28 days of curing (in a membrane of NRVB 20 mm thick, average pressure of 100 kPa) was found to be approximately 2 × 10−15m2in
dry conditions and 5 × 10−17m2in saturated grout (Francis et al.,
1997; Harris et al., 1992). The average pore radius was determined to be 0.45μm, with a pore size distribution ranging from 5 nm to > 1μm (Harris et al., 1992). Harris and colleagues concluded, using the pre-mise that a material is considered to crack if the calculated stress ex-ceeds the tensile strength, that NRVB is able to release gas at a suﬃcient rate without generating cracks (Harris et al., 1992).
implications regarding the applicability of older studies to present day materials in the disposal of nuclear wastes.
2. Materials and methods
Batches of NRVB paste were prepared according to the formulation presented inTable 1, with a water/solid ratio (where solid includes all the powder materials used) of 0.55. It is possible toﬁnd, in the litera-ture, data pertaining to NRVB prepared with laboratory (pure) mate-rials (e.g.Corkhill et al., 2013) and also with industrial materials (e.g. Butcher et al., 2012). To verify the consistency between the cement formed using these two types of starting materials, two diﬀerent bat-ches of NRVB were studied. For the NRVB formulated using laboratory chemicals, denoted NRVB (Lab), the starting materials were: CEM I 52.5 N sourced from Hanson Cement Ltd, Ribblesdale works (i.e. Sellaﬁeld speciﬁcation; BS EN 197-1:2011); Ca(OH)2(≥95.0%) and
CaCO3 (≥99.0%) were sourced from Sigma-Aldrich. In the case of
NRVB formulated using industrial materials, denoted NRVB (Ind), the following products were used: CEM I 52.5 N (as above); hydrated lime sourced from Tarmac Cement & Lime (Tunstead Quarry, Buxton, UK); and limestoneﬂour sourced from National Nuclear Laboratory (Tendley Quarry, Cumbria, UK; BS EN 13043:2002).
The particle size distribution was measured using a Mastersizer
NRVB formulation (Francis et al., 1997; Hooper, 1998).
Material Content (kg m−3)
CEM I 52.5 N 450
Ca(OH)2/Hydrated lime 170
Composition of raw materials, as determined by X-Ray Fluorescence analysis (preci-sion ± 0.1 wt%).
Compound (wt. %)
CEM I 52.5 N
Limestone Flour (Ind)
Hydrated Lime (Ind)
Na2O 0.3 0.2 < 0.1 < 0.1 < 0.1
MgO 1.2 1.6 < 0.1 0.5 0.5
Al2O3 5.2 1.9 < 0.1 < 0.1 0.1
SiO2 19.7 5.4 < 0.1 0.5 0.7
P2O5 0.2 0.1 < 0.1 < 0.1 < 0.1
K2O 0.5 0.3 < 0.1 < 0.1 < 0.1
CaO 64.1 48.1 57.0 73.9 74.5
Fe2O3 2.1 1.7 < 0.1 < 0.1 < 0.1
SO3 – 893 ppm 37 ppm – –
Fig. 1.Particle size distribution of (a) CaCO3and limestoneﬂour and; (b) Ca(OH)2and
Fig. 2.(a) Isothermal calorimetry of NRVB (Lab) and NRVB (Ind). Thermal features identiﬁed are: (1) dissolution and C3A reaction; (2) induction period; (3) reaction of alite
3000 PSA, and the results analysed using Malvern Instruments soft-ware.
The chemical composition of the starting materials, as calculated using X-rayﬂuorescence (PANalytical Zetium XRF) of powdered ma-terials, is shown inTable 2. The composition was very similar for both Ca(OH)2and hydrated lime. However, a slight diﬀerence was observed
between CaCO3 and limestone ﬂour. For example, CaCO3 contained
more CaO than the limestoneﬂour (57 wt% and 48 wt%, respectively). On the other hand, limestone ﬂour presented a higher concentration (between 1.6 and 5.4 wt%) of SiO2, Fe2O3, MgO and Al2O3than reagent
grade CaCO3, which contained below 0.05 wt% of these elements
Both cement batches were mixed using a Kenwood benchtop mixer for 5 min. Subsequently, the cement pastes were placed in centrifuge tubes or steel moulds (for compressive strength analysis) and cured at 20 °C and 95% relative humidity, for 28 days.
2.2. Analytical methods
2.2.1. Mechanical properties
The workability of both NRVB formulations was investigated using a mini-slump test (Kantro, 1980). The cement paste was placed in a cone (19 mm top opening x 38 mm bottom opening x 57 mm height) resting on a sheet of polymethyl-methacrylate. The cone was lifted vertically
upwards and the resulting slump area measured using a scale. Each mini-slump test was repeated in triplicate.
The setting time was ascertained using a Vicatronic automatic re-cording apparatus (Vicat needle method) and 400 g of paste at 19–21 °C and 30–38% relative humidity. The penetration of a needle (1.13 mm diameter) was monitored and the initial setting time was considered as the time when the needle penetration was 35 mm; theﬁnal setting time corresponded to less than 0.5 mm of penetration.
After 28 days of curing, compressive strength was measured on cubes with dimensions of 50 × 50 × 50 mm, in triplicate. Cubes were placed within a Controls Automax automatic compressive tester for analysis, with a loading rate of 0.25 MPa/s. The density of both for-mulations was measured using He pycnometry (Micromeritics AccuPyc II 1340) using approximately 0.40 g of powder (< 63 μm). A ﬁll pressure of 82.7 kPa was purged 50 times over 20 cycles at 25 °C with an equilibration rate of 34.5 Pa/min.
2.2.2. Chemical analysis (hydration)
The heat ﬂow resulting from the NRVB hydration reaction was studied using isothermal calorimetry analysis (TAM Air, TA Instruments) at 20 °C. Approximately 20 g of cement paste was mixed and the measurements were performed for 7 days. As reference sample, tap water was used.
For identiﬁcation of the hydrate phases present in NRVB at an early age (28 days of curing), XRD and TGA-MS were performed on powder samples (< 63μm). The former was carried out using a Bruker D2 Phaser diﬀractometer utilising a Cu Kα source and Ni ﬁlter. Measurements were taken from 5° to 70° 2θwith a step size of 0.02° and 2 s counting time per step. For TG-MS analysis, a PerkinElmer Pyris 1
Fig. 3.X-ray diﬀraction patterns for (a) NRVB (Lab) and NRVB (Ind) after 28 days of curing, and (b) Limestone Flour and CaCO3. Crystalline phases are labelled.
thermogravimetric analyser was used. The temperature ranged from 20 °C to 1000 °C with a heating rate of 10 °C/minute under N2
(ni-trogen) atmosphere. A Hiden Analytical mass spectrometer (HPR-20 GIC EGA) was used to record the mass spectrometric signals for H2O
Scanning Electron Microscopy (SEM) imaging and Energy Dispersive X-ray (EDX) analysis were performed on NRVB monolith samples mounted in epoxy resin and polished to a 0.25μmﬁnish using diamond paste. Backscattered electron (BSE) images were recorded using a Hitachi TM3030 scanning electron microscope operating with an accelerating voltage of 15 kV. EDX analysis was performed using Quantax 70 software and elemental maps were collected for 10 min.
Solid-state nuclear magnetic resonance (NMR) spectra for29Si were collected on a Varian VNMRS 400 (9.4 T) spectrometer at 79.435 MHz
using a probe for 6 mm o.d. zirconia rotors and a spinning speed of 6 kHz, a pulse width of 4μs (90°), a relaxation delay of 2.0 s, and with a minimum of 30000 scans.27Al NMR spectra were collected on the same instrument at 104.198 MHz using a probe for 4 mm o.d. zirconia rotors and a spinning speed of 12 kHz, a pulse width of 1μs (25°), a relaxation delay of 0.2 s, and a minimum of 7000 scans.
2.2.3. Microstructure analysis (porosity)
To determine the Brunauer-Emmett-Teller (BET) surface area, ni-trogen adsorption-desorption measurements were studied at 77 K on a Micromeritics 3 Flex apparatus. Powder samples of raw material were cooled with liquid nitrogen and analysed by measuring the volume of gas (N2) adsorbed at speciﬁc pressures. The pore volume was taken
from the adsorption branch of the isotherm at P/P0= 0.3. Mercury
Fig. 5.BSE SEM micrograph of (a) NRVB (Lab) and (b) NRVB (Ind) at 28 days of curing, with the corresponding EDX maps.
intrusion porosimetry (MIP) was used to study the total porosity and pore distribution of the samples. Small pieces of cement paste were placed into the sample holder of an Autopore V 9600 (Micromeritics Instruments). Washburn's law was used to determine the pore diameter, by applying the following equation: D = (−4cosθ)γ/P, where D is the pore diameter (μm),θthe contact angle between theﬂuid and the pore mouth (°),γthe surface tension of theﬂuid (N/m), and P the applied pressure toﬁll the pore with mercury (MPa). The maximum pressure applied was 208 MPa, the surface tension was 485 mN/m and the contact angle was 130°.
The XCT scans were performed at the University of Strathclyde using a Nikon XTH 320/225 system, equipped with a 225 kV reﬂection gun, a microfocus multimetal target, and a 2000 × 2000 pixel ﬂat panel photodetector (cell size 0.2 × 0.2 mm). The rotation stage po-sition was set so the X-ray source-to sample distance was minimal and allowed a minimum voxel size of 3 micrometres. Scanning conditions were an accelerating voltage of 100 keV, 28μA current (corresponding to power 2.8 W) using a silver target. The exposure time for each projection was 2.829 s, lasting 3141 projections (1 frame per projec-tion) and leading to a scan-time of 2.5 h. Gun conditions would not saturate photodetector, consequently no metallic ﬁlter was required
during the scans. Projections were overlapped in 3 diﬀerent heights of the sample with CT Pro 3D software (©2004–2016 Nikon Metrology) to reconstruct the centre of rotation of the 3D volumes. Once re-constructed, a software built-in algorithmic correction has been applied to correct for artifacts related to beam-hardening (Brooks and Dichiro, 1976). All volumes were reconstructed in 16 bit greyscale, and con-verted to a.tif stack. A volume of interest (VOI) was selected for each sample, using standards previously reported in the literature, i.e. the VOI should be at least 100μm3, or higher than 3 to 5 times the size of
the largest distinct feature, to minimiseﬁnite size error. In this study, the VOI size chosen was 0.42 mm3(250 × 250 x 250 voxels at 3μm resolution).
3. Results and discussion
3.1. Mechanical properties
The workability, determined by mini-slump testing, of NRVB (Lab) and NRVB (Ind) was found to be 56.5 ± 0.8 mm diameter and 68.4 ± 1.7 mm diameter, respectively. The higherﬂuidity of NRVB (Ind) is likely related to the diﬀerence observed in the particle size distribution between the sources of calcium carbonate (Fig. 1a), where 50% of the particles were smaller than 19.7μm for CaCO3, and 11.5μm
for limestone ﬂour. For laboratory and industrial grade Ca(OH)2
(Fig. 1b), the particle size distribution was found to be very similar. For general applications, the initial setting time of a cement should not be less than 45 min, and theﬁnal setting time should not be greater than 10 h (Bensted and Barnes, 2008; Taylor, 1997). Using the Vicat method, it was possible to obtain an initial setting time of 5.3 h, and a ﬁnal setting time of 7.7 h for NRVB (Lab). For NRVB (Ind) the values were very similar, with the initial andﬁnal setting times at 5.5 h and 7.3 h. This is in contrast to the initial NRVB formulation study, where an initial setting time of 4.05 h and aﬁnal setting of 4.50 h was ob-served (Francis et al., 1997). Since the w/s ratio in the present study is the same as that used byFrancis et al. (1997), this diﬀerence is likely to be related to the use of diﬀerent raw material, and a consequent dif-ference in the reactivity of the materials.
After 28 days of curing, the compressive strength and density of the two materials were compared. The compressive strength was de-termined to be 8.2 ± 0.2 MPa for NRVB formulated using laboratory materials and 7.15 ± 0.04 MPa for NRVB formulated with industrial materials. This is somewhat greater than that measured byFrancis et al. (1997), who found a compressive strength of 5.9 MPa at 28 days for NRVB prepared using components available in the early 1990s. Since no characterisation of these starting materials was published, it is not possible to ascertain which component of this early NRVB formulation gave rise to the reduced strength, although it may be postulated that the 52.5 MPa grade cement used in our trials was of a higher strength grade than the materials used historically, as cement production at this high strength grade was much less common in the early 1990s. The density was determined by helium pycnometry to be 2.251 ± 0.001 g/cm3for
NRVB (Lab) and 2.328 ± 0.002 g/cm3 NRVB (Ind); previous
mea-surements of NRVB density using the Archimedes method (100 mm cubes) gave a density of 1.7 g/cm3in water-saturated NRVB samples and 1.1 g/cm3in oven dried samples (Francis et al., 1997). This lower
value could reﬂect the diﬀerence in the methodology used; the Archi-medes method determines bulk density, whereas pycnometry allows the determination of solid density as helium gas reaches all of the pores within the cement.
3.2. Chemical analysis (hydration)
Fig. 2a shows the isotherm generated for both NRVB formulations during hydration. It is possible to identify the four main hydration stages, as observed in a plain Portland cement. In comparison to Port-land cement, the heat ﬂow was lower (Fig. 2b) by a factor of ∼2
Fig. 7.27Al MAS NMR spectra of NRVB (Lab) and NRVB (Ind) after 28 days of curing.
(Jansen et al., 2012). This is related to the much lower fraction of material undergoing hydration in the NRVB formulation. Comparing the two formulations of NRVB, it can be observed that the heatﬂow was very similar, however one subtle diﬀerence was observed: the curve corresponding to the sulfate depletion period (labelled 4,Fig. 2a) of NRVB (Ind) indicates that it evidenced a more intense reaction than NRVB (Lab). One possible explanation is the formation of additional calcium monocarboaluminate hydrate in NRVB (Ind) as observed in XRD and NMR data (discussed below). In accordance with the particle size analysis (Fig. 1a), determination of the surface area of the CaCO3
sources indicated that the limestone ﬂour used in NRVB (Ind) had a signiﬁcantly higher surface area than CaCO3used in NRVB (Lab), with
values of 5.2 ± 0.2 m2/g and 3.7 ± 0.2 m2/g, respectively. The higher surface area is responsible for a higher rate of calcite dissolution and also the availability of more nucleation sites, resulting in the for-mation of more hydration products (Scrivener et al., 2015). Another factor to consider is the higher content of sulfate present in the in-dustrial raw material, which may give rise to the observed diﬀerences; the limestoneﬂour of NRVB (Ind) had 893 ppm sulfur, compared with
37 ppm in the hydrated lime of NRVB (Lab) (Table 2).
The main phases identiﬁed in the NRVB formulations by X-ray Diﬀraction (XRD) were calcite (CaCO3; PDF 01-086-0174) and
por-tlandite (Ca(OH)2; PDF 01-072-0156) (Fig. 3a). Ettringite
(Ca6Al2(OH)12(SO4)3·26H2O; PDF 00-041-1451), calcium
mono-carboaluminate hydrate (Ca4Al2(OH)12(CO3)3·5H2O; PDF 01-087-0493)
and calcium hemicarboaluminate hydrate (Ca4Al2(OH)12 [OH
(CO3)0.5]·5.5H2O; PDF 00-041-0221) were also identiﬁed. These results
are in agreement with those identiﬁed previously in NRVB cured at ambient temperature (Felipe-Sotelo et al., 2012). While the phase as-semblage for each formulation was similar, subtle diﬀerences were observed in the peak intensities of several reﬂections; mono-carboaluminate reﬂections were more intense in NRVB (Ind) than NRVB (Lab), while reﬂections of calcite were more intense in NRVB (Lab), which is also apparent in the XRD patterns corresponding to limestoneﬂour and CaCO3(Fig. 3b). These diﬀerences may be
attrib-uted to the chemical composition, particle size distribution and surface area of the CaCO3and limestoneﬂour, however, preferential
orienta-tion cannot be ruled out, especially for layered or platy phases such as
monocarboaluminate and portlandite.
TG-MS analysis conﬁrmed the presence of the phases identiﬁed by XRD (Fig. 4). The two peaks between 100 and 200 °C can be attributed to the presence of ettringite and monocarboaluminate, while the peaks between 400 and 500 °C, and 650–800 °C correspond to portlandite and calcite, respectively (Lothenbach et al., 2007; Sun, 2011). The same peaks were observed for both formulations, however for the NRVB (Ind) (Fig. 4b) an additional peak was observed at∼650 °C, corresponding to the presence of magnesian calcite and supported by the presence of a greater quantity of Mg in NRVB (Ind) than NRVB (Lab) (Table 2).
Through SEM imaging and EDX analysis it was possible to identify the microstructure of the diﬀerent hydrate phases, as shown inFig. 5. The large Ca-containing rhombohedral crystals (labelled A,Fig. 5) are portlandite. The Ca and Si-rich phase surrounding portlandite crystals (labelled B, Fig. 5) may be C-S-H. The areas containing higher con-centrations of aluminium (labelled C,Fig. 5) suggest the presence of AFm phases. The areas labelled D are indicative of the presence of sulfate-containing AFm phases and/or ettringite, due to the higher concentration of both aluminium and sulfate. Comparing the SEM images of the two formulations, it is possible to identify the same hy-drate phases, however the matrix of NRVB formulated with industrial materials has a more ﬁne grained morphology, consistent with the analysis of limestoneﬂour.
In the29Si MAS NMR spectra (Fig. 6) it was possible to identify some unreacted Portland cement through the presence of alite (chemical shifts−69 and−73.9 ppm) and belite (−71.2 ppm) (Scrivener et al., 2016) in both NRVB formulations. Contributions from Q1(−79 ppm), Q2(1Al) (−83 ppm) and Q2(−84 ppm) silicate environments were also
observed in both formulations; these chemical shifts are characteristic of C-S-H (Richardson, 2008; Richardson et al., 2010). A small resonance was also observed at−90 ppm corresponding to Q3(1Al). The presence of Al shows the incorporation of this element in the C-(A)-S-H (Richardson et al., 2010). Comparison of the two formulations reveals a small diﬀerence in the spectra (Fig. 6a and b) between NRVB (Lab) and NRVB (Ind); this is related to the intensity of Q2(−84 ppm), Q2(1Al)
(−83 ppm) and Q3(1Al) (−90 ppm). A possible reason is the diﬀerence
observed in the reactivity of the raw materials used in the two for-mulations, speciﬁcally the higher surface area of the limestoneﬂour.
Fig. 7shows the27Al NMR spectra of NRVB (Lab) and NRVB (Ind).
The small peak observed at approximately−69 ppm (more evident for NRVB Ind) is attributed to the substitution of Al for Si in C-S-H (Lothenbach et al., 2008), in agreement with the observation of small peaks corresponding to Q2(1Al) and Q3(1Al) in the29Si MAS NMR
spectra (Fig. 6). The peaks visible at approximately +13 and + 9 ppm indicate the presence of octahedrally coordinated Al in ettringite and AFm phases. As stated previously in the literature (Lothenbach et al., 2008), it is not possible to distinguish between the diﬀerent AFm phases due to the similar chemical shift. Comparing the two formulations, it is possible to see a diﬀerence in the proportion of ettringite and AFm phases present; the presence of more AFm in NRVB (Ind) is related to the higher availability of dissolved carbonate (higher surface area) and consequent formation of monocarboaluminate, in accordance with the results observed by isothermal calorimetry (Fig. 2a) and XRD (Fig. 3a). 3.3. Microstructure (porosity)
A two-fold approach was applied to determine the porosity of the two NRVB formulations, to ensure all pore sizes were considered in the analysis. Mercury Intrusion Porosimetry, where it is understood that the pore diameters obtained correspond to the pore entry size and not the real size of the pore (Scrivener et al., 2016), was performed to compare the trend and changes in the pore size distribution between the two NRVB formulations (Diamond, 2000).Fig. 8shows the pore entry size diameter in relation to the cumulative intrusion for NRVB (Lab) and NRVB (Ind). The curve for NRVB (Lab) allocates essentially all of the pores to threshold pore entry radii below 0.8 μm, whereas for NRVB
(Ind) the curve allocates all of the pores to sizes below 0.5μm. This small diﬀerence is also evident in the total porosity obtained, where for NRVB (Lab) the percentage of total porosity obtained was 38 ± 1% and for NRVB (Ind) was 32 ± 1%. It is important to note that, due to the low compressive strength of NRVB (around 8 MPa), this technique (which reaches pressures of 208 MPa in the instrument used in this study) might not be suitable to use to quantify theﬁner pores due to the potential for collapse of pores during analysis. This is expected to occur at∼0.14 mL/g of intrusion for NRVB (Lab) and at∼0.15 mL/g for NRVB (Ind) based on the strength data.
X-ray Computed Tomography was also used to study the porosity of NRVB. This technique has the advantage of being non-invasive and to allow three-dimensional reconstructions, but has limitations in spatial resolution.Fig. 9shows selected slices of the VOI for the two samples analysed. Quantitative analysis was performed using segmentation of the VOI. A threshold value was chosen based on the line shape of the image histograms, which show peaks of higher and lower absorption voxels, where the lower absorption voxels correspond to surrounding air and internal void space (Landis and Keane, 2010), allowing dis-crimination between pore space and binder phases (solid). The MIP results were used to guide the thresholding process, so the comparison between the results obtained by the two techniques is to some degree inﬂuenced by this.
No cracks were observed in the samples at this early age (28 days of hydration). The porosities obtained from tomographic data were 39% for NRVB (Lab) and 35% for NRVB (Ind). This diﬀerence is related, once more, to the diﬀerence observed in the hydration reaction of both ce-ments, due to the smaller particle size and higher surface area of limestoneﬂour.
The porosity results are in the same range presented byHeyes et al. (2015)(∼40%), however they are lower than those reported byFrancis et al. (1997), where the porosity measured using MIP and nitrogen desorption was around 50%. It is important to note, however, that by estimating the porosity using the density values measured in Francis et al. (∼35%), the results obtained in this paper are very similar. Dif-ferences in the characteristics between the raw materials used in the 1990's and those used in the present study are likely to be responsible for the diﬀerences observed.
3.4. Inﬂuence of precursor materials on NRVB characteristics and properties
In summary, the diﬀerences in the surface area and chemical com-position of the raw materials, particularly CaCO3and limestoneﬂour,
impacted the properties of the NRVB formulations. In addition to dif-ferences between the NRVB formulations investigated here, we also observed diﬀerences between the results obtained in this study when compared to the characterisation performed in the early 1990's, likely due to diﬀerences in the raw material and other unspeciﬁed properties. The impact of raw material selection on properties required for geolo-gical disposal are discussed below.
Workability, compressive strength and setting time were aﬀected by the use of diﬀerent raw materials. In the present study, the higher surface area of limestoneﬂour resulted in a higher workability and lower compressive strength for NRVB formulated with industrial raw materials when compared to NRVB formulated with laboratory raw materials. When comparing our data with those from the early 1990's (Francis et al., 1997), the workability and setting time were a factor of ∼1.5 lower in the present study, which we attribute to diﬀerences in ﬁneness of the precursor materials used. The diﬀerences observed should not strongly inﬂuence the ability for the backﬁll to be poured within vaults, and the compressive strength values obtained are low enough to allow re-excavation of the vaults if necessary.
material. In the present study, the rate of hydration was faster in NRVB formulated with industrial raw materials due to the high surface area of limestoneﬂour. The quantity of monocarboaluminate was also greater, which is a consequence of the higher availability and reactivity of dissolved carbonate in limestoneﬂour. Furthermore, small diﬀerences in the chemical composition of limestoneﬂour, for example, the pre-sence of S (and, to a lesser extent, Mg) inﬂuenced the rate of hydration. This may have implications for the hydrate phase assemblage at time-scales longer than 28 days of curing; further work is required to in-vestigate this.
Through 29Si MAS NMR spectroscopy we have shown the in-corporation of aluminium in the C-(A)-S-H of NRVB, and that the choice of raw material inﬂuences the quantity incorporated (Figs. 6 and 7). Previous studies have shown that aluminium incorporated into amor-phous silica reduces the dissolution rate, even in high alkaline en-vironments (Chappex and Scrivener, 2013, 2012; Iler, 1973). Therefore, the buﬀering behaviour of the repository may not occur on the pre-dicted time scale, or result in a pH comparable to that estimated when considering C-S-H dissolution only (Nuclear Decommissioning Authority, 2010b).
Finally, we observed that the choice of raw material also inﬂuences the 28-day porosity of the ﬁnal NRVB, which is associated with the diﬀerences in hydration reaction outlined above; the formation of more hydrate products in NRVB formulated with industrial materials resulted in a slightly lower porosity. In a repository environment, such a dif-ference may strongly inﬂuence the rate of groundwater ingress and the egress of gas, which are key design functions of NRVB.
The use of diﬀerent raw materials in the synthesis of NRVB has been investigated, and the diﬀerences in workability, setting time, hydration and porosity analysed. These results are compared with those pre-viously reported in the literature for this material, and the potential eﬀects of diﬀerences in raw materials on the ﬁnal use of NRVB have been explored. Surface area,ﬁneness and chemical composition of the raw materials, particularly limestoneﬂour, have been shown to inﬂu-ence, to a small extent,ﬁnal backﬁll properties including setting time, compressive strength and buﬀering capacity. The eﬀects on porosity seem to be signiﬁcant, but this may also be due to diﬀerences in ana-lysis techniques applied to investigate this property. This study high-lights the importance of a detailed characterisation of raw materials used in the formulation of NRVB for use in a geological disposal facility, especially in light of concerns surrounding security of cement supply for future applications.
The authors wish to acknowledge funding for this research from Radioactive Waste Management and the European Commission Horizon 2020 Research and Training Programme, Cebama, of the European Atomic Energy Community (EURATOM), under grant agreement number 662147. CLC also wishes to acknowledge EPSRC for the award of an ECR Fellowship (EP/N017374/1). This research was performed in part at the MIDAS Facility, at the University of Sheﬃeld, which was established with support from the Department of Energy and Climate Change. Solid-state NMR spectra (27Al, 29Si) were obtained at the EPSRC UK National Solid-state NMR Service at Durham, and we thank Dr. David Apperley for his assistance in collection and interpretation of the results. X-ray microtomography is funded by the Scottish Funding Council's Oil and Gas Innovation Centre.
Bamforth, P.B., Baston, G.M.N., Berry, J.A., Glasser, F.P., Heath, T.G., Jackson, C.P., Savage, D., Swanton, S.W., 2012. Cement materials for use as backﬁll, sealing and
structural materials in geological disposal concepts. In: A Review of Current Status. SERCO/005125/001 Issue 3.
Bensted, J., Barnes, P., 2008. Structure and Performance of Cements, second ed. Taylor & Francis e-Library.
Brooks, R., Dichiro, G., 1976. Beam hardening in X-ray reconstructive tomography. Phys. Med. Biol. 390–398.
Butcher, E.J., Borwick, J., Collier, N., Williams, S.J., 2012. Long term leachate evolution duringﬂow-through leaching of a vault backﬁll (NRVB). Mineral. Mag. 76, 3023–3031.http://dx.doi.org/10.1180/minmag.2012.076.8.18.
Chappex, T., Scrivener, K.L., 2013. The eﬀect of aluminum in solution on the dissolution of amorphous silica and its relation to cementitious systems. J. Am. Ceram. Soc. 96, 592–597.http://dx.doi.org/10.1111/jace.12098.
Chappex, T., Scrivener, K.L., 2012. The inﬂuence of aluminium on the dissolution of amorphous silica and its relation to alkali silica reaction. Cem. Concr. Res. 42, 1645–1649.http://dx.doi.org/10.1016/j.cemconres.2012.09.009.
Corkhill, C.L., Bridge, J.W., Chen, X.C., Hillel, P., Thornton, S.F., Romero-Gonzalez, M.E., Banwart, S. a., Hyatt, N.C., 2013. Real-time gamma imaging of technetium transport through natural and engineered porous materials for radioactive waste disposal. Environ. Sci. Technol. 47, 13857–13864.http://dx.doi.org/10.1021/es402718j. Crossland, I.G., Vines, S.P., 2001. Why a cementitious repository. Nirex Report N/034. Diamond, S., 2000. Mercury porosimetry: an inappropriate method for the measurement of pore size distributions in cement-based material. Cem. Concr. Res. 30, 1517–1525. http://dx.doi.org/10.1016/S0008-8846(00)00370-7.
Felipe-Sotelo, M., Hinchliﬀ, J., Evans, N., Warwick, P., Read, D., 2012. Sorption of radionuclides to a cementitious backﬁll material under near-ﬁeld conditions. Mineral. Mag. 76, 3401–3410.http://dx.doi.org/10.1180/minmag.2012.076.8.53. Francis, A.J., Cather, R., Crossland, I.G., 1997. Nirex Safety Assessment Research
Programme: Development of the Nirex Reference Vault Backﬁll; Report on Current Status in 1994. Report no: S/97/014..
Harris, A.W., Atkinson, A., Claisse, P.A., 1992. Transport of gases in concrete barriers. Waste Manag. 12, 155–178.
Harris, A.W., Manning, M.C., Tearle, W.M., Tweed, C.J., 2002. Testing of models of the dissolution of cements - leaching of synthetic CSH gels. Cem. Concr. Res. 32, 731–746.http://dx.doi.org/10.1016/S0008-8846(01)00748-7.
Heyes, D.W., Butcher, E.J., Borwick, J., Milodowski, A.E., Field, L.P., Kemp, S.J., Mounteney, I., Bernal, S.A., Corkhill, C.L., Hyatt, N.C., Provis, J.L., Black, L., 2015. Demonstration of carbonation of the NRVB. Natl. Nucl. Lab. 16 NNL (14) 13296 Issue 4.
Hicks, T.W., Baldwin, T.D., Hooker, P.J., Richardson, P.J., Chapman, N.A., McKinley, I.G., Neall, F.B., 2008. Concepts for the Geological Disposal of Intermediate-level Radioactive Waste. Report no. 0736–1. pp. 1–66.
Hoch, A.R., Baston, G.M.N., Glasser, F.P., Hunter, F.M.I., Smith, V., 2012. Modelling evolution in the nearﬁeld of a cementitious repository. Mineral. Mag. 76, 3055–3069.http://dx.doi.org/10.1180/minmag.2012.076.8.21.
Holland, T.R., Tearle, W.M., 2003. Serco assurance a review of NRVB mineralogy. Serco Assur SERCO/ERRA-0455 January.
Hooper, A.J., 1998. Repository for radioactive waste-vault backﬁll. Patent number: 5,740, 546.
Iler, R.K., 1973. The eﬀect of particle size on the solubility of amorphous silica in water. J. Phys. Chem. 43, 399–408.http://dx.doi.org/10.1021/j150557a024.
Jansen, D., Goetz-Neunhoeﬀer, F., Lothenbach, B., Neubauer, J., 2012. The early hy-dration of Ordinary Portland Cement (OPC): an approach comparing measured heat
ﬂow with calculated heatﬂow from QXRD. Cem. Concr. Res. 42, 134–138.http://dx. doi.org/10.1016/j.cemconres.2011.09.001.
Kantro, D.L., 1980. Inﬂuence of water reducing admixtures on properties of cement paste - a Miniature Slump Test. Cem. Concr. Aggregates 2, 95–102.
Landis, E.N., Keane, D.T., 2010. X-ray microtomography. Mater. Charact. 61, 1305–1316. http://dx.doi.org/10.1016/j.matchar.2010.09.012.
Lothenbach, B., Le Saout, G., Gallucci, E., Scrivener, K., 2008. Inﬂuence of limestone on the hydration of Portland cements. Cem. Concr. Res. 38, 848–860.http://dx.doi.org/ 10.1016/j.cemconres.2008.01.002.
Lothenbach, B., Winnefeld, F., Alder, C., Wieland, E., Lunk, P., 2007. Eﬀect of tempera-ture on the pore solution, microstructempera-ture and hydration products of Portland cement pastes. Cem. Concr. Res. 37, 483–491.http://dx.doi.org/10.1016/j.cemconres.2006. 11.016.
Menéndez, G., Bonavetti, V., Irassar, E.F., 2003. Strength development of ternary blended cement with limestoneﬁller and blast-furnace slag. Cem. Concr. Compos 25, 61–67. http://dx.doi.org/10.1016/S0958-9465(01)00056-7.
Nuclear Decommissioning Authority, 2015. Geological Disposal the 2013 Derived Inventory. Report no. NDA/RWM/120..
Nuclear Decommissioning Authority, 2010a. Geological Disposal: an Overview of the Generic Disposal System Safety Case. NDA Report no. NDA/RWMD/010.. Nuclear Decommissioning Authority, 2010b. Geological Disposal: Near-ﬁeld Evolution
Status Report. Report no. NDA/RWMD/033. Nuclear Decommissioning Authority. Nuclear Decommissioning Authority, 2010c. Retrievability of Waste Emplaced in a
Geological Disposal Facility. Doc No RWMDPP03 December. Nuclear Decommissioning Authority.
Radioactive Waste Management, 2016. RWM HAW Innovation and Delivery: a Review of Cement Powders Security of Supply, Speciﬁcations and Disposability Issues. Report no. NDA/RWM/144. Nuclear Decommissioning Authority.
Richardson, I.G., 2008. The calcium silicate hydrates. Cem. Concr. Res. 38, 137–158. http://dx.doi.org/10.1016/j.cemconres.2007.11.005.
Richardson, I.G., Black, L., Skibsted, J., Kirkpatrick, R.J., 2010. Characterisation of ce-ment hydrate phases by TEM, NMR and Raman spectroscopy. Adv. Cem. Res. 22, 233–248.http://dx.doi.org/10.1680/adcr.2010.22.4.233.
Analysis of Cementitious Materials. CRC Press, Taylor & Francis Group. Scrivener, K.L., Juilland, P., Monteiro, P.J.M., 2015. Cement and concrete research
ad-vances in understanding hydration of Portland cement. Cem. Concr. Res.http://dx. doi.org/10.1016/j.cemconres.2015.05.025.
Sun, J., 2011. Carbonation Kinetics of Cementitious Materials Used in the Geological Disposal of Radioactive Waste. PhD thesis. . http://discovery.ucl.ac.uk/1306875/.
Swanton, S.W., Heath, T.G., Clacher, A., 2016. Leaching behaviour of low Ca:Si ratio CaO–SiO2–H2O systems. Cem. Concr. Res. 88, 82–95.http://dx.doi.org/10.1016/j. cemconres.2016.06.001.
Taylor, H.F. (Ed.), 1997. Cement Chemistry, second ed. Thomas Telford Publishing. United Kingdom Nirex Limited, 2005. Context Note 4.1: Retrievability. United Kingdom